Active Standard ASTM C191 | Developed by Subcommittee: C01.30
Book of Standards Volume: 04.01
Historical (view previous versions of standard)
Significance and Use
This test method provides a means of determining compliance with a specification limit for Vicat time of setting. Refer to the appropriate specification for the cement to determine if this test method is used for specification compliance.
Time of setting measured by this method will not necessarily provide the same results as the time of setting of hydraulic cement paste measured by other methods, or the time of setting of mortar or concrete.
1.1 These test methods determine the time of setting of hydraulic cement by means of the Vicat needle. Two test methods are given; Method A is the Reference Test Method using the manually operated standard Vicat apparatus, while Method B permits the use of an automatic Vicat machine that has, in accordance with the qualification requirements of this method, demonstrated acceptable performance.
1.2 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.3 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. See 1.4 for a specific warning statement.
1.4 Warning—Fresh hydraulic cementitious mixtures are caustic and may cause chemical burns to skin and tissue upon prolonged exposure. The use of gloves, protective clothing, and eye protection is recommended. Wash contact area with copious amounts of water after contact. Wash eyes for a minimum of 15 min. Avoid exposure of the body to clothing saturated with the liquid phase of the unhardened material. Remove contaminated clothing immediately after exposure.
1.5 The text of this standard references notes and footnotes which provide explanatory material. These notes and footnotes (excluding those in tables and figures) shall not be considered as requirements of the standard.
Note 1—For the method for determining the time of setting by Gillmore needles, see Test Method C 266
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C150 Specification for Portland Cement
C151 Test Method for Autoclave Expansion of Hydraulic Cement
C183 Practice for Sampling and the Amount of Testing of Hydraulic Cement
C187 Test Method for Amount of Water Required for Normal Consistency of Hydraulic Cement Paste
C219 Terminology Relating to Hydraulic Cement
C266 Test Method for Time of Setting of Hydraulic-Cement Paste by Gillmore Needles
C305 Practice for Mechanical Mixing of Hydraulic Cement Pastes and Mortars of Plastic Consistency
C511 Specification for Mixing Rooms, Moist Cabinets, Moist Rooms, and Water Storage Tanks Used in the Testing of Hydraulic Cements and Concretes
C595 Specification for Blended Hydraulic Cements
C1005 Specification for Reference Masses and Devices for Determining Mass and Volume for Use in the Physical Testing of Hydraulic Cements
C1157 Performance Specification for Hydraulic Cement
D1193 Specification for Reagent Water
ICS Number Code 91.100.10 (Cement. Gypsum. Lime. Mortar)